### Ultrafast and Distinct Spin Dynamics in Magnetic Alloys

I. Radu*,†,**,††_{, C. Stamm}†,‡‡_{, A. Eschenlohr}†,§§_{, F. Radu}‡_{, R. Abrudan}§_{,}
K. Vahaplar*_{, T. Kachel}†_{, N. Pontius}†_{, R. Mitzner}†_{, K. Holldack}†_{, A. F}€ohlisch†_{,}

T. A. Ostler¶, J. H. Mentink*_{, R. F. L. Evans}¶_{, R. W. Chantrell}¶_{,}
A. Tsukamoto||, A. Itoh||,A. Kirilyuk*_{, A. V. Kimel}*_{and Th. Rasing}*

*Radboud University, Institute for Molecules and Materials Heyendaalseweg 135, 6525 AJ Nijmegen, The Netherlands

†_{Institut f}_{€ur Methoden und Instrumentierung}
der Forschung mit Synchrotronstrahlung

Helmholtz-Zentrum Berlin f€ur Materialien und Energie GmbH Albert-Einstein-Straße 15, 12489 Berlin, Germany

‡_{Institut f}_{€ur Komplexe Magnetische Materialien}

Helmholtz-Zentrum Berlin f€ur Materialien und Energie GmbH Albert-Einstein-Straße 15, 12489 Berlin, Germany

§_{Institut f}_{€ur Experimentalphysik/Festk€orperphysik}
Ruhr-Universit€at Bochum, 44780 Bochum, Germany

¶_{Department of Physics, University of York}
Heslington, York YO10 5DD, United Kingdom

||_{College of Science and Technology}

Nihon University, 7-24-1 Funabashi, Chiba, Japan
**_{radu@tu-berlin.de}

Received 23 May 2015 Accepted 26 May 2015 Published 20 August 2015

Controlling magnetic order on ultrashort timescales is crucial for engineering the next-generation magnetic devices that combine ultrafast data processing with ultrahigh-density data storage. An appealing scenario in this context is the use of femtosecond (fs) laser pulses as an ultrafast, external stimulus to fully set the orientation and the magnetization magnitude of a spin ensemble.

**_{Corresponding author.}

††_{Currently with the Institute for Optics and Atomic Physics Technical University Berlin, Germany.}

‡‡_{Currently with the Department of Material Science, ETH Zürich Schafmattstr. 30, 8093 Zürich, Switzerland.}

§§_{Currently with Fakultät für Physik, Universität Duisburg-Essen Lotharstr. 1, 47057 Duisburg, Germany.}

This is an open access article published by World Scienti¯c Publishing and distributed under the terms of the Creative Commons Attribution (CC BY) 4.0 License, which permits use, distribution and reproduction in any medium, provided the original author(s) and source are credited.

Vol. 5, No. 3 (2015) 1550004 (10 pages)

*© The Authors*

DOI:10.1142/S2010324715500046

Achieving such control on ultrashort timescales, e.g., comparable to the excitation event itself, remains however a challenge due to the lack of understanding the dynamical behavior of the key parameters governing magnetism: The elemental magnetic moments and the exchange interaction. Here, we investigate the fs laser-induced spin dynamics in a variety of multi-com-ponent alloys and reveal a dissimilar dynamics of the constituent magnetic moments on ultrashort timescales. Moreover, we show that such distinct dynamics is a general phenomenon that can be exploited to engineer new magnetic media with tailor-made, optimized dynamic properties. Using phenomenological considerations, atomistic modeling and time-resolved X-ray magnetic circular dichroism (XMCD), we demonstrate demagnetization of the constituent sub-lattices on signi¯-cantly di®erent timescales that depend on their magnetic moments and the sign of the exchange interaction. These results can be used as a \recipe" for manipulation and control of magnetization dynamics in a large class of magnetic materials.

Keywords: Ultrafast spin dynamics; element-speci¯c magnetization; atomistic spin simulations.

1. Introduction

Femtosecond (fs) laser-induced controlling of
fer-romagnetic order1 _{has intrigued researchers since}
the pioneering work of Beaurepaire et al.,2 _{who}
found that fs optical excitation of ferromagnetic Ni
can demagnetize the sample on a sub-picosecond
time-scale. This demagnetization event was much
faster than one might expect supposing that the
demagnetization process is de¯ned by the
charac-teristic time of the spin-lattice relaxation in the
ground state. Later, it was demonstrated that
cir-cularly polarized laser pulses could act as equally
short and relatively strong e®ective magnetic ¯eld
pulses,3 _{even leading to fs laser-induced switching}
of the magnetization.4 _{These intriguing }
observa-tions have triggered intense experimental and
the-oretical e®orts to understand the fundamental
processes underpinning such ultrafast laser-induced
dynamics.1 Although a few models of laser-induced
demagnetization of simple ferromagnets such as Ni,
Fe, Co and Gd have been suggested,5–7 _{the physics}
of ultrafast magnetic phenomena in systems with
two or more magnetic sublattices8–13 _{still }
chal-lenges our understanding. Yet many magnetization
dynamics studies were performed with magnetic
compounds containing at least two magnetic
ele-ments, like the well-known Permalloy,14–16 _{}
ortho-ferrites,3 _{manganites}17 _{and yttrium}_{–iron–garnets.}18
In the conventional macrospin approximation,1 _{the}
constituent magnetic sublattices of an alloy are
represented by a single macrospin [see Fig. 1(a)],
which is used to describe their static and dynamic
properties. This implies that two exchange-coupled
magnetic sublattices are dynamically
indistin-guishable and thus would lose their magnetization

on the very same time-scale upon ultrafast (fs)
laser excitation. However, recent experiments using
fs X-ray magnetic circular dichroism (XMCD)
have revealed distinctly di®erent magnetization
dynamics of the constituent magnetic moments in
a Gd(FeCo) alloy excited by a fs optical pulse.10
Moreover, it was subsequently shown19 _{that these}
distinct dynamics in combination with the
ex-change interaction between the sublattices, can
lead to a deterministic switching of this
ferrimag-netic Gd(FeCo) by an ultrafast heat pulse alone.20
These results lead to the intriguing question of
whether such element-speci¯c spin dynamics is a
general phenomenon or something strictly related

(a) (b)

Fig. 1. Schematic illustration of the conventional (a) and of the ultrafast and distinct (b) spin dynamics. In the conventional picture (a) the dynamics of spin systems consisting of several magnetic elements is treated in the macrospin approximation where all the constituent elements are treated as a single mac-rospin. Within the ultrafast and distinct spin dynamics picture (b), one accounts for the dynamics of each magnetic constituent of a multi-component magnetic alloy separately, their dynamics being governed by the magnitude of their magnetic moment (the arrows in the ¯gure) and by their mutual exchange inter-action (the springs in the ¯gure).

to a narrow class of GdFe-like ferrimagnetic materials?

Here, we investigate the dynamics of multi-sub-lattice magnetic materials with both ferromagnetic and antiferromagnetic coupling between their sub-lattices. Using phenomenological modeling and atomistic spin simulations, we show that their de-magnetization dynamics is distinct and element-speci¯c. These simulations are fully supported by element-speci¯c fs time-resolved XMCD experi-ments on various NiFe and rare earth-transition metal (RE-TM) alloys, which provide evidence for a demagnetization time that scales with the elemental magnetic moment and varies with the sign of the exchange interaction. As such, one can tune the speed of magnetization processes in multi-sublattice alloys by properly choosing the magnitude of the constituent magnetic moments and the sign of the exchange interaction that couples them. These results may lead to new design principles of mag-netic media for fast and energy-e±cient magmag-netic data manipulation and storage.12,13,23

2. Phenomenological Model of Ultrafast Magnetization

Dynamics in Ferromagnetic Alloys

To gain a qualitative understanding of the ultrafast
demagnetization dynamics in ferromagnetically
or-dered two-sublattice magnets, we employ a
macro-scopic theory developed originally by Baryakhtar21
for the description of the dynamics and relaxation of
the macroscopic (sublattice) magnetization of
fer-romagnets and antiferfer-romagnets. It was recently
shown that this approach can qualitatively describe
the spatially averaged and dominantly longitudinal
dynamics obtained from atomistic spin dynamics
simulations.8 _{Clearly, the Baryakhtar theory is not}
restricted to longitudinal dynamics, and it has
re-cently been demonstrated22 _{for antiferromagnetic}
coupling in the exchange approximation, that in
addition to the purely longitudinal solutions, the
theory exhibits a second class of solutions, which for
speci¯c conditions allows for the appearance of
transverse time evolution with the same timescale as
the longitudinal exchange relaxation. For the
pres-ent work, we are interested in a di®erpres-ent regime,
where both the relativistic relaxation as well as the
exchange relaxation play an important role (regime
3 according to Ref.8), and we will restrict ourselves

to the class of longitudinal solutions only. This approach is supported by atomistic simulations,23 which show that even when the system exhibits a small canting before laser excitation, the fast initial relaxation directly after excitation, i.e., the ultrafast demagnetization, is dominantly longitudinal. Fur-thermore, all experiments that operate at macro-scopic length scales, including the X-ray experiments we describe below, demonstrate a longitudinal evolution of the (sublattice) magnetization on the sub-picosecond timescale. Hence on macroscopic length scales, the longitudinal time-evolution seems to be the relevant one. Under these conditions, the equations of motion are:

_S1¼ 1H1þ eðH1 H2Þ; ð1aÞ
_S2¼ 2H2þ eðH2 H1Þ; ð1bÞ
where Si denotes the macroscopic spin angular
mo-mentum of sublattice i¼ 1; 2, and Hi ¼ W=Siis
the e®ective magnetic ¯eld for sublattice i, which is
derived from the magnetic (Landau) free energy W.
i are the relativistic relaxation parameters
de-scribing the transfer of angular momentum with
the environment, while e describes the exchange
relaxation responsible for transfer of angular
mo-mentum between the sublattices. Previous work8
considered both _{i;e} and the free energy W as
phe-nomenological parameters. As a next step, to assess
the in°uence of the concentration, we derive
the macroscopic free energy from a microscopic
Heisenberg model, which is also the basis for
atom-istic spin dynamics simulations. Hence, similar to
the latter, we explicitly assume that the longitudinal
time-evolution on the macroscopic scale originates
from spatial averaging over the transverse dynamics
of the atomistic spins. Using the methods described
in e.g., Refs. 24–26, we obtain in the mean ¯eld
approximation for classical spins and for small Si
values:
W ¼ _{2N}1
11S
2
1þ_{2N}1
22S
2
2_{N}2Np
1N2J12S1S2;
ð2aÞ
1i ¼ 3
2
1
k_{B}T 2ziiJii: ð2bÞ
For a binary alloy, we can use N_{1}¼ ð1 xÞN,
N_{2}¼ xN, Np¼ xð1 xÞzN, z11¼ z21¼ ð1 xÞz,
z_{22}¼ z12¼ xz, where x is the concentration of
sub-lattice 2, z the average number of nearest neighbors

in the alloy, and N the total number of spins per unit
volume. In addition, i indicates the magnitude of
the spin angular momentum in sublattice i and Jij
are exchange parameters between spins in sublattice
i and j that we take for nearest neighbors only.
Further, k_{B}T is the energy of the temperature
°uc-tuations experienced by the spins, which we assume
to be solely determined by the electron temperature.
In principle, it is possible to extract the relaxation
parameters from microscopic theory in a similar
way as ¯rst-principle calculations of the
trans-verse Gilbert relaxation parameter.27,28 _{This will}
generally yield parameters that depend on the
temperature, the exchange interactions and the
concentration. Below, we will consider the
relaxa-tion parameters_{i;e} as purely phenomenological, in
order to gain qualitative understanding in the limits
of small and large concentration.

To understand qualitatively how the
demagneti-zation time changes by going from the pure element
to the alloy, we consider ¯rst the limiting case of
small x. In this limit, we simplify the theory using
eðxÞ i for x 1 and the transfer of angular
momentum between the sublattices will in general
be a small e®ect. Furthermore, this transfer is
gen-erally less e®ective for ferromagnetic coupling than
for antiferromagnetic coupling, since the terms in
H_{1} H2 partly cancel each other. Therefore, we
can write the demagnetization rate after a (fs
laser-induced) step-like change of the electron
tempera-ture as _S_{1}¼ _{1}H_{1}. Using Eqs. (2a) and (2b) with
S_{1}jt¼0¼ N11ðxÞ we ¯nd:

_S1ðxÞ ¼ 1ðxÞ½3kBT ð1 xÞzJ11 xzJ12=1ðxÞ:
ð3Þ
As in the pure material, we ¯nd a demagnetization
time that depends on the magnetic moment, and
hence the Ni and Fe sublattices generally have
dis-tinct dynamics after laser excitation due to the
dif-ference in their magnetic moments. In addition, the
concentration determines the sublattice magnetic
moments and exchange coupling strength, which
can be di®erent from the pure material. This in turn
leads to a change in demagnetization times
com-pared to the pure material. Applying this to the
NiFe alloy at small Fe concentration, we have
J_{NiNi} < JNiFe.29Since alsoNið0Þ < NiðxÞ30(see also
Supplementary Sec. 6), we anticipate the
de-magnetization time of Ni increases upon moderate
doping with Fe.

Next, we investigate the limit of large
con-centration (x 0:5). As before, the relativistic
contributions generally yield distinct dynamics,
however the transfer of angular momentum between
the sublattices may not be negligible anymore. For
example, at high-temperature (k_{B}T Jij) we have
H_{1} H2 3kBT ð11 12 Þ ¼ þ3kBT ð1 2Þ=
12. The sign of this term depends on the di®erence
1 2, which suggests an additional acceleration
(deceleration) of sublattice 1 (2) when _{1}< _{2}.
Unfortunately, it is not straightforward to apply
this analysis to the case of NiFe, since for large
concentration the system is in the Invar region. In
this regime, the Ni sublattice remains almost
col-linear with the average magnetization, but the Fe
sublattice is essentially frustrated and noncollinear
even at very low temperature. This frustration is
caused by long-range oscillating exchange
interac-tions31 _{and due to local environment e®ects that}
yield a huge dispersion of the nearest-neighbor
ex-change parameters,32 _{which results in a decrease of}
the Curie temperature despite the fact that the
magnitude of the exchange interactions increases.33
Although the assessment of such frustrated
magne-tism goes beyond the nearest-neighbor Heisenberg
model employed here, we anticipate that an
essen-tially noncollinear Fe environment can allow for an
e±cient transfer of angular momentum between
the sublattices (large parameter eÞ, which in the
high-temperature limit yields an acceleration of the
demagnetization of Ni, since_{Ni}< _{Fe}. This
accel-eration counteracts the decelaccel-eration due to the
in-crease of _{Ni}, which in the Invar regime is almost
twice as large as in pure Ni. Hence, the exchange
relaxation in the Invar regime can make the
dy-namics of Ni and Fe more distinct than anticipated
solely from the di®erence of the magnetic moments,
which is indeed the trend observed in the atomistic
and experimental results shown below.

3. Atomistic Spin Simulations of Ultrafast Demagnetization

Following the model predictions above, we have performed atomistic simulations of the response of 106 ferromagnetically exchange-coupled NiFe as well as antiferromagnetically coupled GdFe spins to an ultrashort 60 fs heat pulse, as explained in the Supplementary Information. The dynamics of each magnetic sublattice were obtained by solving a

system of coupled stochastic Landau–Lifshitz–
Gilbert equations for individual atomic moments,
which describe the transient dynamics of the system
upon excitation with a fs laser pulse.34 _{For}
multi-component magnetic alloys one derives34,35 _{a}
characteristic longitudinal relaxation timea (i.e.,
demagnetization time) for each constituent
compo-nent which scales with:

i i

2iikBT ; ð4Þ
wherei is the moment associated with site i; i is
the coupling constant to the thermal bath,i is the
gyromagnetic ratio at site i, k_{B} is Boltzmann's
constant and T is the temperature of the bath.
Consequently, if an alloy consists of two sublattices
and _{16¼}_{2}, a rapid heating of the system to high
temperatures will lead to di®erent demagnetization
dynamics of the two sublattices, despite the strong
exchange interaction that couples them. The e®ect
ofiandion the demagnetization time is discussed
in Supplementary Sec. 7.

We have simulated both ferromagnetically
pled NiFe alloys as well antiferromagnetically
cou-pled GdFe (ferrimagnetic) systems. Following
Ref.34, we coupled the spin system to the electron
temperature that is calculated using the
two-temperature model,36 _{which describes the transient}
variation of the electron and phonon temperatures
upon femtosecond laser excitation. The strength of
the thermal °uctuations then scales with this
time-varying temperature. For simplicity, the model
assumes the same coupling constants for the
di®er-ent sublattices (i¼ 0:01), and the magnetic
moments were derived from XMCD measurements
(see Supplementary Information). The NiFe
ex-change interactions were determined from the
measured Curie temperature of the NiFe alloy
samples as reported in Ref.37. For instance, in the
case of Ni_{50}Fe_{50}, this yields a total exchange per spin
of 260 meV. The results of the Ni_{50}Fe_{50} simulations
are displayed in Fig. 2(a), showing clearly a faster
demagnetization for Ni than for Fe. This conclusion
holds for the full stoichiometry range of the NiFe
alloys, as detailed in the Supplementary Sec.6.

To simulate the antiferromagnetically coupled GdFe system, we used the exchange constants obtained by ¯tting the temperature-dependent

XMCD data measured for the Fe and Gd
sub-lattices.35_{Taking into account the number and type}
of neighbors, the total e®ective Fe–Gd exchange is
30 meV. The results of the GdFe simulations are
displayed in Fig. 2(b), showing a dissimilar
demag-netization dynamics of Fe and Gd with Fe being
much faster than Gd.

Hence, distinct timescales for the demagnetiza-tion of magnetic sublattices have been computed for both ferromagnetic and antiferromagnetic coupling between the sublattices. Thus, this appears to be a general phenomenon for multi-sublattice magnets.

(a)

(b)

Fig. 2. Computed transient dynamics of the constituent
magnetic moments in FeNi and GdFe alloys using the atomistic
spin model. The response of the longitudinal component of the
magnetization of Ni and Fe in Ni_{50}Fe_{50}alloy (a) and of Fe and
Gd in Gd_{24}Fe_{76}alloy (b) to a 60 fs laser pulse. The dashed lines
in both panels display the transient electronic temperature used
in the simulation. The starting temperature for the simulation is
300 K. Note that in panel (b) the Fe and Gd curves are merging
together around 1.8 ps (see Supplementary Information Sec.3).

a_{The longitudinal relaxation time denotes here the decay of the z component of the volume-averaged magnetic moment (whose}

length is locally conserved).

4. Ultrafast Dynamics of the Elemental Magnetic Moments from

Time-Resolved XMCD Experiments

To compare these theoretical predictions and
simulations with experiments, we measured the
transient demagnetization dynamics of the
mag-netic sublattices in NiFe and GdFe alloysbas well as
their respective pure elements, employing the
ele-ment-speci¯c XMCD technique in transmission at
the femto-slicing facility38,39 of the Helmholtz–
Zentrum Berlin. In addition, we have also
investi-gated a ferrimagnetic DyCo5 (i.e., Dy16:7Co83:3)
alloy40_{that shows the largest di®erence between the}
magnitudes of the constituent magnetic moments
(see Supplementary Fig. 3). The experiments were
performed in a stroboscopic pump-and-probe mode,
where the metallic samples were excited with 60 fs
laser pulses of 1.55 eV photon energy. Subsequent
laser-induced magnetization dynamics were probed
by measuring the XMCD changes in transmission
with circularly polarized 100 fs X-ray pulses39_{tuned}
at the L3 edges of Ni (853 eV), Fe (707 eV), Co
(778 eV) and at the M5 edges of Gd (1189 eV) and
Dy (1292 eV). At these energies, we probe the
dy-namics of the 3d magnetic moment of Ni, Fe, Co
and the 4f moment of Gd and Dy, respectively. We
point out that at these absorption edges, there is a
nonambiguous relationship between the measured
XMCD signal and the elemental magnetic
moments41 _{that remains valid even in the high}
nonequilibrium regime after laser excitation.42 _{The}
XMCD measurements were performed on Fe, Ni,
Ni_{50}Fe_{50}, Ni_{80}Fe_{20}, Dy_{16:7}Co_{83:3} and Gd_{25}Fe_{66}Co9
samples at 300 K except for DyCo5, which were
done at 100 K (under laser exposure the e®ective
sample temperature of DyCo5 rose well above its
compensation temperature of 120 K due to a
per-manent heating e®ect, as deduced from the polarity
of the XMCD signal and the elemental hysteresis).
For Gd(FeCo), the magnetization compensation
temperature was 250 K. The typical absorbed
laser °uence was 6.8 mJ/cm2 for NiFe alloys,
10.1 mJ/cm2

for DyCo5 while for Gd(FeCo) it was 4.5 mJ/cm2. The Fe, Ni and NiFe ¯lms exhibit an in-plane magnetization orientation, while Gd(FeCo) and DyCo5 have an out-of-plane mag-netic anisotropy. The samples are poly-crystalline except for Gd(FeCo) which is amorphous.

The results of the element-speci¯c laser-induced
demagnetization of ferromagnetic Ni_{50}Fe_{50} are
shown in Fig. 3(a). Upon fs laser excitation, the
alloy demagnetizes to about 50% at both the Fe and
Ni edges. Although a similar degree of
demagneti-zation is achieved for both elements, their transient
demagnetization behavior is considerably di®erent:
While Fe is demagnetized within 800 fs, it takes
only 300 fs for Ni to demagnetize to the same
extent as Fe, in qualitative agreement with the

(a)

(b)

Fig. 3. Element-speci¯c demagnetization dynamics of the
constituent magnetic moments in FeNi and GdFe alloys
measured by time-resolved XMCD with fs time-resolution.
El-ement-speci¯c demagnetization measured in (a) ferromagnetic
Ni_{50}Fe_{50}at the Fe L3and Ni L3edges and (b) in ferrimagnetic

Gd_{25}Fe_{66}Co9alloy at the Fe L3and Gd M5edges. The solid lines

are ¯ts according to a bi-exponential ¯t function (see Eq. (5)). The Gaussian pro¯les depict the time resolution of the XMCD measurements of 130 fs.

b_{The GdFe sample contained a small percentage (9%) of Co to control the magnetic anisotropy}_{— for more details, see }

Supple-mentary Information Sec. 1.

predictions from Fig. 2(a). Although less
pro-nounced, we measure similar distinct
demagnetiza-tion dynamics of the Fe and Ni moments in a
Ni_{80}Fe_{20}sample with again Fe being slower than Ni
(see Supplementary Fig. 7).

Essentially, a similar decoupled demagnetization behavior of the constituent, but antiferromagneti-cally coupled, magnetic moments is encountered for the ferrimagnetic Gd(FeCo) alloy, as shown in Fig. 3(b). In this case, the demagnetization of Fe takes 400 fs while Gd demagnetizes within 1.2 ps. Due to the lower TC of 550 K (see Ref.35), here we totally quench the magnetic order at both Fe and Gd edges i.e., achieve a demagneti-zation degree of 100%. This dynamic decoupling of Fe and Gd is however also encountered for much lower demagnetization degrees down to 40% (see Supplementary Fig. 8).

For the ferrimagnetic alloy DyCo5, according to Eq. (4) and given the di®erent values of the con-stituent Co ( 1.52 B) and Dy ( 8.91 B) magnetic moments (see Supplementary Fig. 3), we expect a large di®erence between their dynamics. Indeed, as shown in Supplementary Fig. 9, Co demagnetizes down to 50% within 350 fs while it takes several ps for Dy to reach the same demagnetization level.

To extract the time constants of the measured demagnetization transients, we have used the fol-lowing bi-exponential ¯t function:

fðtÞ ¼ gðtÞ
A B exp _{}t
D
þ C exp _{}t
R
;
ð5Þ
where D and R are the demagnetization and
relaxation time constants, g(t) is the Gaussian
function describing the time resolution of the
ex-periment, B and C are the exponential amplitudes
and A is the value of the transient signal at negative
delays. The demagnetization time constants
obtained from the ¯ts are listed in Table 1 of
Sup-plementary Information and plotted in Fig. 4(a).
For comparison, we also show the demagnetization
time constants of the elemental Fe, Ni, Co and Gd
samples. The demagnetization of pure Co and Gd
are taken from Refs. 5 and 43, respectively. For
demagnetization of pure Ni, please see also Ref. 44.
We note that these demagnetization time constants
are extracted from demagnetization transients (both

the alloys and their elemental counterparts) that
exhibit similar demagnetization degreesM=M_{0} of
around 50%, and thus we can treat and compare
these demagnetization times on equal footing. In
Fig. 4(b) we show the deduced demagnetization
constants versus magnetic moment for all measured
samples. One observes a clear scaling behavior
be-tween the demagnetization time and the magnitude
of the magnetic moment. A quantitative estimate
for the variation of the demagnetization time per
magnetic moment unit is obtained by ¯tting the

(a)

(b)

Fig. 4. The experimental demagnetization time constants
measured for single Ni, Fe, Co and Gd elements and their alloys.
In panel (a), we show the overview of the demagnetization time
constants of the elemental magnetic moments in the Ni_{80}Fe_{20},
Ni_{50}Fe_{50}, DyCo5and Gd25Fe66Co9alloys and of the pure Fe, Ni,

Co and Gd samples. The solid lines are guides to the eye. De-magnetization time constants of pure Co and Gd are taken from Refs.5and43, respectively, while the demagnetization of Co in CoPd alloy is taken from Ref.45. The gray regions emphasize the dissimilar demagnetization time constants of the elements in the same alloy. Panel (b) shows the dependence of the demag-netization time constants from panel (a) on the magnitude of the elemental magnetic moments for pure elements and their alloys. The solid line is a linear ¯t to the data.

data using a linear ¯t function [the solid line in Fig.4
(b)], which gives us a value of90 20 fs/_{B}.

Another important piece of information provided by these data is the dependence of the demagneti-zation time on the magnetic ordering type of the samples. This is shown in Fig. 5 where the demag-netization time constants of Fe and Co are plotted for pure samples, ferromagnetic FeNi and CoPd and ferrimagnetic (i.e., antiferromagnetic coupling) Gd (FeCo) and DyCo alloys. For a ferromagnetic type of coupling, both the Fe and Co moments demag-netize slower than the pure material while the op-posite is observed in the antiferromagnetically coupled GdFe and DyCo. Please note that the very same behavior is encountered when normalizing the elemental demagnetization times to the corre-sponding magnetic moment magnitudes.

5. Discussion

There are three major e®ects that can be observed in the overview of the demagnetization time constants shown in Figs. 4 and 5: (i) The distinctly di®erent demagnetization times of the elemental magnetic moments in the ferromagnetic NiFe and ferrimag-netic Gd(FeCo) and DyCo5 alloys [the highlighted regions in Fig.4(a)], (ii) the demagnetization times scale approximately with the magnitude of the ele-mental magnetic moment [see Fig.4(b)] for the pure samples of Ni, Fe, Co and Gd as well as for their alloys and (iii) the demagnetization time of a speci¯c element (e.g., Fe or Co) changes with the exchange

interaction type of the host alloy i.e., it is longer in ferromagnetic FeNi and shorter in antiferro-magnetically coupled Gd(FeCo) and DyCo5 com-pared to their pure Fe and Co counterparts (see Fig.5).

Both the XMCD data and the simulations show that, despite the strong ferromagnetic exchange coupling between the Ni and Fe sublattices in NiFe, they apparently lose their net magnetization in a very dissimilar manner. The same situation is also observed in ferrimagnetic Gd(FeCo) and DyCo5, where two antiferromagnetically coupled Gd and Fe or Dy and Co sublattices demagnetize on substan-tially di®erent time-scales. Thus, we observe the same transient decoupling of the exchange-coupled magnetic moments in two material systems that are strikingly di®erent, i.e., ferromagnetic versus anti-ferromagnetic coupling, itinerant versus localized type of magnetic ordering and in-plane versus out-of-plane magnetic anisotropy. Consequently this distinct dynamics seems to be a general property of multi-elemental magnetic compounds that are driven nonadiabatically to a highly nonequilibrium state by fs laser excitation. Moreover, in agreement with Eqs. (3) and (4), the observed characteristic demagnetization times scale with the magnetic moment of the sublattices i.e., the larger the mag-netic moment the slower the demagnetization pro-cess [see Fig. 4(b)]. For the materials investigated here, we obtain a characteristic change of the demagnetization time per magnetic moment of 90 20 fs/B. Consequently, although in NiFe, Fe demagnetizes slower than Ni, in Gd(FeCo) the de-magnetization of the Fe-sublattice is much faster than the demagnetization of Gd. This distinct dy-namics is even more pronounced in DyCo5given the large di®erence (a factor of 6) between the Dy and Co magnetic moments.

Furthermore, the antiferromagnetic coupling in
Gd(FeCo) and DyCo5yields faster demagnetization
of both sublattices when compared to their pure
elements. The ferromagnetic coupling in Ni_{50}Fe_{50},
on the other hand, yields faster demagnetization of
Ni and slower demagnetization of Fe, despite the
fact that the magnetic moment of Ni increases
(see Supplementary Fig. 3 for variation of the
magnetic moment with the sample stoichiometry).
In Ni_{80}Fe_{20}, the exchange coupling between the
sublattices is not e®ective enough (see Table 2 in
Supplementary Information) to compensate for the
increased magnetic moment, yielding an increase of
Fig. 5. The dependence of the demagnetization times for Fe

and Co on the magnetic ordering type of the host alloys. Comparison of the demagnetization time constants measured for Fe and Co in ferromagnetic FeNi and CoPd, ferrimagnetic GdFeCo and DyCo as well as for pure elements. The demag-netization time constants for pure Co and Co in CoPd are taken from Refs.5and45, respectively.

the demagnetization time of Ni compared to the pure case.

Overall, these results show that is possible to control the dynamics of the constituent sublattices in magnetic alloys by changing the magnitude of the magnetic moment of the constituent elements, the sign and strength of the exchange interaction or a combination thereof. Moreover, knowing the key parameters that govern the ultrafast magneti-zation dynamics in alloys, we can extend this \recipe" and hypothesize that magnetization dy-namics can be engineered the very same way in arti¯cial magnetic structures mimicking the intrinsic properties of alloys, as for instance in synthetic ferrimagnets.46

Before concluding the paper, we would like to
discuss the relevance of the recent transversal
mag-neto-optical Kerr e®ect (TMOKE) results by
Mathias et al.15 _{in the context of our study. These}
authors used time-resolved magneto-optics in
re-°ection to investigate the laser-induced
demagneti-zation of pure Fe, Ni and of a permalloy (Ni_{80}Fe_{20})
sample. By tuning the probing VUV photon energy
at the M_{3;2} (3p–3d transitions) resonances of Ni
( 67 eV) and Fe ( 54 eV) they report that Fe
demagnetizes quicker than Ni in pure samples
while in Permalloy both elements exhibit the same
demagnetization time (about 240 fs) and a time lag
in the onset of their respective transient dynamics.
There are two major di®erences between our work
and the study of Ref. 15: (i) Their measurements
were performed in re°ection geometry and
(ii) magnetization dynamics has been probed at the
M_{3;2} elemental edges in the VUV spectral range.
Regarding point (i), magneto-optical X-ray
mea-surements performed in re°ection do not provide a
direct, quantitative measure of the elemental
mag-netic moment, which is at variance compared to
their transmission counterparts.41 _{This is because}
the magneto-optical signal measured in re°ection
consists of an admixture of dispersive and absorptive
parts of the dielectric function, and as such the use of
the sum rulescto determine the magnetic moment is
inapplicable. Second, in the VUV spectral range the
energies corresponding to the spin-orbit and the
exchange interactions are of comparable magnitude,
which leads to a strong distortion of the 3p electronic
states of Ni and Fe (the M3and M2absorption edges

are essentially overlapped) and consequently, one cannot apply the sum rules to obtain the magnitude of the magnetic moment (see e.g., Ref. 47). This is valid for both re°ection and absorption measure-ments. Moreover, in the VUV range, the close en-ergetic proximity of Fe and Ni absorption edges results in an overlap of their respective magnetic signals; this renders, for such alloys, the interpreta-tion of the magnetizainterpreta-tion data in terms of pure ele-mental response more di±cult and ambiguous. Also, the time-resolved TMOKE measured in the VUV range might be susceptible to magneto-optical arti-facts, as has been recently pointed out by Vodungbo et al.48 Thus, the TMOKE signal might contain nonmagnetic contributions that complicate the in-terpretation of the data as being only of magnetic origin.

In short, due to their measurement speci¯city, the
results of Mathias et al.15 _{do not provide }
informa-tion about the dynamics of the elemental magnetic
moment in their samples. This is at variance with
our present work performed in the soft X-ray
spec-tral range, which allows the accurate application of
the magneto-optical sum rules and thus providing a
nonambiguous relationship between the measured
signal and the magnetic moment. As such, there is
no common basis for comparing our results with
those reported in Ref.15 as this work is essentially
measuring di®erent observables.

6. Conclusion

To conclude, our atomistic spin modeling and phe-nomenological theory, supported by element-speci¯c fs XMCD experiments, demonstrate the possibility of tuning the dynamics of multi-sublattice ferro-magnets and ferriferro-magnets by their composition, which determines their magnetic moments and the strength of the exchange interaction. This can lead to distinctly di®erent demagnetization times even for the same element in di®erent alloys. In particu-lar, we have shown that for antiferromagnetic coupling, exchange relaxation accelerates the de-magnetization of both sublattices, while with ferro-magnetic coupling, the dynamics of one sublattice is accelerated while the other is slowed down. Fur-thermore, we have shown that, by tuning the com-position we can control the distinctiveness of the

c_{The magneto-optical sum rules relate the absorption cross-section with the ground-state expectation values of the spin}_{hS}_{z}_{i and}

orbitalhLzi moments.
SPIN Downloaded from www.worldscientific.com _{by 81.151.46.168 on 08/20/15. For personal use only.}

sublattice dynamics. This allows designing new magnetic materials, for example using exchange coupled multilayers, which combine desirable prop-erties for future recording media.12,13,23

Acknowledgments

Funding from the European Community's Seventh Framework Program (FP7/2007–2013) Grants No. NMP3-SL-2008-214469 (UltraMagnetron), No. 214810 (FANTOMAS) and No. 281043 (FEMTOSPIN) and ERC Grant No. 257280 (Femtomagnetism) as well as Grant No. 226716 and ERC-2013-AdG339813-EXCHANGE, the German Federal Ministry of Education and Research (BMBF) Grant No. 05K10PG2 (FEMTOSPEX), the Foundation for Fundamental Research on Matter (FOM) and the Netherlands Organization for Scienti¯c Research (NWO) is gratefully acknowledged.

References

1. A. Kirilyuk, A. V. Kimel and Th. Rasing, Rev. Mod. Phys. 82, 2731 (2010).

2. E. Beaurepaire, J.-C. Merle, A. Daunois and J.-Y. Bigot, Phys. Rev. Lett. 76, 4250 (1996).

3. A. V. Kimel et al., Nature (London) 429, 850 (2004). 4. C. D. Stanciu et al., Phys. Rev. Lett. 99, 047601

(2007).

5. B. Koopmans et al., Nature Mater. 9, 259 (2010). 6. M. Battiato, K. Carva and P. M. Oppeneer, Phys.

Rev. Lett. 105, 027203 (2010).

7. J.-Y. Bigot, M. Vomir and E. Beaurepaire, Nature Phys. 5, 515 (2009).

8. J. Mentink et al., Phys. Rev. Lett. 108, 057202 (2012).

9. S. Wienholdt et al., Phys. Rev. B. 88, 020406 (2013). 10. I. Radu et al., Nature (London) 472, 205 (2011). 11. N. Bergeard et al., Nature Commun. 5, doi: 10.1038/

ncomms4466 (2014).

12. S. Mangin et al., Nature Mater. 13, 286 (2014). 13. C. H. Lambert et al., Science 345, 1337 (2014). 14. C. La-O-Vorakiat et al., Phys. Rev. Lett. 103,

257402 (2009).

15. S. Mathias et al., P. Natl Acad. Sci. USA 109, 4792 (2012).

16. I. Radu et al., Phys. Rev. Lett. 102, 117201 (2009). 17. T. Lottermoser et al., Nature 430, 541 (2004). 18. S. O. Demokritov et al., Nature 443, 430 (2006). 19. T. Ostler et al., Nature Commun. 3, 666 (2012). 20. J. Barker et al., Scienti¯c Reports 3, 03262 (2013). 21. V. G. Baryakhtar Sov. Phys. JETP 60, 863 (1984). 22. V. G. Baryakhtar, V. I. Butrim and B. A. Ivanov,

JETP Lett. 98, 289 (2013).

23. R. Evans et al., Appl. Phys. Lett. 104, 082410 (2014).

24. H. Falk, Am. J. Phys. 38, 858 (1970).

25. O. F. Abubrig et al., Physica A 296, 437 (2001). 26. J. W. Negele and H. Orland, Quantum

Many-Particle Systems (Westview Press, Boulder USA, 1988).

27. H. Ebert et al., Phys. Rev. Lett. 107, 066603 (2011). 28. A. A. Starikov et al., Phys. Rev. Lett. 105, 236601

(2010).

29. P. Yu et al., Phys. Rev. B 77, 054431 (2008). 30. B. Glaubitz et al., J. Phys.: Condens. Matter 23,

254210 (2011).

31. M. van Schilfgaarde et al., Nature 400, 46 (1999). 32. A. V. Ruban et al., Phys. Rev. B 71, 054402 (2005). 33. J. Kudrnovský et al., Phys. Rev. B 77, 224422

(2008).

34. N. Kazantseva et al., Europhys. Lett. 81, 27004 (2008).

35. T. Ostler et al., Phys. Rev. B. 84, 024407 (2011). 36. S. I. Anisimov, B. L. Kapeliovich and T. L.

Perel-man, Sov. Phys. JETP 39, 375 (1974).

37. E. H. Wasserman, in Ferromagnetic Materials, Vol. 5 (Elsevier, Amsterdam , The Netherlands, 1990). 38. C. Stamm et al., Nature Mater. 6, 740 (2007). 39. S. Khan et al., Phys. Rev. Lett. 97, 074801 (2006). 40. F. Radu, R. Abrudan, I. Radu, D. Schmitz and H.

Zabel, Nature Commun. 3, 715 (2012).

41. C. T. Chen et al., Phys. Rev. Lett. 75, 152 (1995). 42. K. Carva et al., Europhys. Lett. 86, 57002 (2009). 43. M. Wietstruk et al., Phys. Rev. Lett. 106, 127401

(2011).

44. C. Stamm et al., Phys. Rev. B 81, 104425 (2010). 45. C. Boeglin et al., Nature 465, 458 (2010).

46. R. Evans, T. Ostler, R. Chantrell, I. Radu and
Th. Rasing, Appl. Phys. Lett. 104, 082410 (2014).
47. D. Zhao et al., J. Appl. Phys. 84, 2858 (1998).
48. B. Vodungbo et al., Phys. Rev. X 3, 038001 (2013).
SPIN Downloaded from www.worldscientific.com _{by 81.151.46.168 on 08/20/15. For personal use only.}